SMEAR LAYER • Introduction
• Components of smear layer
• Bonding and smear layer
• Functional Implications
• Methods of Removal
INTRODUCTION: Unknown and unrecognized for years, the smear layer has become a force to be reckoned with during the last decade. The full significance
has been slow
interest in adhesive bonding to tooth structure.
Its effect as a
so called “Cavity liner” is just beginning to be appreciated. As suggested by David Pashley, the smear layer as a cavity liner may unquestionably have both beneficial and deterimental effects. Thus there is a need to alter the traditional procedures of restorative treatment to take advantage of the beneficial effects and to avoid the detrimental effects. DEFINITION: I.
According to Operative Dentistry Journal (1984) the term smear layer applies to “any debris produced introgenically by the cutting, not only of dentin, but also of enamel, cementum and even the dentin of the root canal”.
Cohen defined smear layer as “an amosphous, relatively smooth layer of microcrystalline debris whose featureless surface cannot be seen with the naked eye”.
III. The American Association of Endodontists defined smear layer as a “surface film of debris retained on dentin or other
endodontic files”. IV. According to DCNA (1990) when tooth structure is cut, instead of being uniformly sheared, the mineralised matrix 2
Existing of the strategic interface of restorative
materials and the dentin matrix most of the debris is scattered over the enamel and dentin surface to form what is known as smear layer. HISTORY: The earliest studies on the effects of various instruments on dental tissues were those reported by Lammie and Draycott in 1952 and Stret (1953).
These attempts were limited
principally to light microscope. Charbeneou, Peyton and Anthony were among the first to quantify and rank the differences b/w burs and abrasives by using a prolifometer to record the surface topography of cut and abraded dental tissues. In
microscopy to study the nature of the cut tooth surface. It was not until the advent of SEM that the grinding debris was first referred to as the smear layer by Boyde, Switsur and Stewart in 1963 and further defined by Eick and others in 1970, who referred to it as the smear layer. In 1972, Jones, Lozdan and Boyde showed that smear layers were common on enamel and dentin following the use of periodental instruments. Eick and others in 1970 attempted to quantify and identify cutting debris on tooth surfaces. They confirmed that: •
Surfaces abraded with diamonds were rougher than those cut with tungsten carbide burs. 3
Surfaces cut dry were rougher and more smeared than those in which water was used as coolant.
The smear layer is composed of an organic film less than 0.5 mm thick.
Included with in it were particles of
opacity ranging from 0.5 – 15 mm.
Such layer were
present on all surfaces though they were not necessarily continuous. In 1982, Goldman and others studied smear layers after the use of endodontic instrumentation. Erich and co-workers in 1976 discussed the role of friction and abrasion in the drilling of teeth. They accounted for the formation of smear layers, especially in dentin by a brittle and ductile transition and alternating rupture and transfer of apatite and collagen matrix into the surface. COMPONENTS OF SMEAR LAYER: The exact proportionate composition of the smear layer has not been determined but SEM examinations have disclosed that its composition is both organic and inorganic. The inorganic material in the smear layer is made up of tooth
contaminants. The organic components may consist of heated co-agulated proteins,
processes plus saliva, blood cells and microorganisms. THE SMEAR PHENOMENON:
In a dental content Eirich in 1976 stated that smearing occurs when “hydroxy apacite within the tissue is either pluncked out or broken or swept along and resets in the smeared out matrix”. Studies have shown that temperature will rise upto 600 o C in dentin when it is cut without a coolant.
This value is
significantly lower than the melting point of apatile (15001800 o C) and has led most to conclude that smearing is a physico-chemical
transformation of apatite involving mechanical shearing and thermal dehydration of the protein.
Plastic flow of hydroxy
apatite is believed to occurs at lower temperature than its melting point and may also be a contributing factor to smearing. MORPHOLOGY OF THE SMEAR LAYER: The smear layer consists of two separate layers, a superficial layer and a layer loosely attached to the underlying dentin. Dentin debris enters the orifices of the dentinal tubules and acts as plugs to occlude the ends of the tubules. The smear layer
continuous over the substrate.
Smear layers found on deep
dentin contain more organic material than those found on the superficial dentin. Clinically produced smear layers have an average depth of from 1-5 mm (Goldman et.al. 1981, Mader et.al. 1984).
depth entering the dentinal tubule may vary from a very few mm to 40 mm. Cengiz et.al. (1990) proposed that the penetration of smear layer into dentinal tubules could be caused by capillary action as a result of adhesive forces b/w the dentinal 5
tubules and the smear material. One can conclude that a smear layer is present on all restoratively or endodontically prepared teeth unless the dentin surface was treated with an acid or chelating agent. Several factors may cause the depth of the smear layer to vary from tooth to tooth: a. Dry or wet cutting of the dentin. b. The type of instrument used and c. The amount solution. Filing spray use of use of
a canal without irrigation or cutting without a water will produce a thicker layer of dentin debris and the coarse diamond burs produces a smear layer than the carbide burs.
The differences in topographical detail after cutting dentin and enamel with steel and tungsten burs and abrading it with the diamond stons are clearly evident. Steel and tungsten carbide burs produce an undulating pattern, the trough of which run perpendicular with the direction of movement of the hand piece. Fine grooves can be seen running perpendicular to the undulations and parallel with the direction of rotation of the bur. Such a phenomenon is referred to as “galling” and the frictional humps represents a “rebound effect” of the burs against the tissue. The galling phenomenon appears more masked with tungsten carbide burs run at high spee. An examination of both steel and tungsten carbide burs shows a rapid determination of the cutting edges through what appears to be a brittle. Brittle significantly deminishes the cutting effeciency of the bur, probably increases frictional heat and causes smearing. Steel and tungsten carbide burs at higher magnification can be seen to have obliterated the normal structural detail of 6
Debris, irregular in shape and non-uniform in
size and distribution, remains on the surface even after thorough lavage with H 2 O. ďƒ˜ The
by which burs remove dental tissue is
significantly different from the abrading action of a diamond. As burs rotate, the flute undermines the tissue, the amount being determined by such factors as the angle of attack of the flute.
On the other hand, abrasive particles, passing
across the tissue, plough throughs in which substrate is ejected ahead of the abrading particle and elevated into ridges
Several factors govern the size of the grooves, including particle size, pressure and hardness of the abrasive related to the substrate.
Diamonds Diamonds produce relative deep and uniform grooves. Produce more rougher surface.
Steel & Tungsten carbide burs Shows less evidence of grooves. Produce less rougher surface compared to diamond.
The grooves run parallel with
Grooves run perpendicular
the direction of motion of
with the direction of motion of
Coarse diamond abrasives used dry produce the thickest deposits. A significant difference exists between diamond burs used with and without coolant or water spray.
In the absence of
coolant smeared debris does not form a continuous layer but 7
exists rather as localised islands with discontinuities exposing the underlying dentin.
Coolant of the water spray does not
prevent smearing but appear to significantly reduce the amount and distribution of it. BONDING THE SMEAR LAYER: In general diamonds, through the introduction of grooved anomalies, produce a greater surface area than burs.
increased surface area probably offers a large number of retentive
micromechanical and the retention mechanism for the tissue lies in the multitude of superficial micropores enhanced following acid conditioning of the tissue. Acids are among several agents that can remove the smear layer.
For enamel H 3 PO 4 phoshoric acid in gel solution
ranging from 30-50% is most popular.
Wall and Cwinett demonstrated that conditioning facilities the penetration of resin into the dentinal tubules. This increases bond strength. FUNCTIONAL IMPLICATIONS: 1. DENTAL MATERIALS: Dental material scientists have been concerned about the smear layer in so far as it masks the underlying dentin matrix and may interface with the bonding of adhesive dental cements such as polycarboxylates and g/c which may react chemically with the dentin matrix. Presumably allowing cements to react chemically with the smear layer rather than with the matrix of sound tubular dentin produces a weaker bond due to the fact that the smear layer can be torn away from the underlying matrix. 8
When cements are applied to dentin covered with a smear layer and then tested for tensile str, the failure can be adhesive (b/w cement and smear layer) or cohesive (b/w constituents of smear layer). 2. RESTORATIVE DENTISTRY: Viewed in this theoretical perspectives if one could produce a truly adhesive filling material that had no shrinkage upon polymerisation and a co-efficient of thermal expansion close to that of tooth structure, then one would want to remove the smear layer and omit the use of any cavity liner or varnish that did not react chemically with both dentin and the resin. There are three possible routes for microleakage. •
With in or via the smear layer.
Between the cavity varnish / cement and the restorative material. At numerous points with in such a complex 3D structure,
the 3 routes interesect permitting microbial products access to dentinal tubules and underlying pulp. The question of microleakage of restorative materials is beyond the scope.
It is worth mentioning however, that there
are at least 2 or 3 routes by which subs can leak into the pulp. First, even if there were no gap b/w dentin and restorative material bacterial products could theoretically diffuse around the matrix via small channels and interstices within the smear layer.
Unfortunately one cannot perfectly adapt amalgam or
any other restorative mat to the walls of a prepared cavity. Thus there are voids and spaces b/w amalgam and dentin that 9
allow considerable microleakage. Most clinicians use a cavity varnish or liner to seal dentin. I. INFLUENCE
SENSITIVITY OF DENTIN: Etching the dentin of roots, whether done therapeutically or by the action of micro-org of plaque can remove the thin layer of covering cementum or smear layer or both conditioning with acids will remove the smear layer plugs exposing patent dentinal tubules to the oral cavity. This can lead to sensitivity of the dentin to the point where it interferes with the pats oral hygiene. Several studies indicate that most of the resistance to the flow of fluid across dentin is due to the presence of smear layer.
Etching dentin greately increases the ease which fluid
can move across dentin.
This is accompanied clinically by
increased sensitivity of dentin to cosmotic, thermal and tactile stimuli. II. INFLUENCE ON THE PERMEABILITY OF DENTIN: Substances
proportional to their concentration gradient and the surface available for diffusion. The
permeability by 5-6 times invitro by diffusion but increases it by 25-36 times by filtration. Diffusion
Filtration / Convection 10
Transport of mat through
Occurs from areas of higher
dentin is due to the presence
convection to lower.
of a pressure gradient. There is no change in the convection of substances dissolved in the fluid as the
The convection of substances
fluid and all that is dissolved
is dissipated over a distance.
in it is made to flow from one point to another. The driving force is pressure.
Thus movement of fluid across dentin by convection is much more sensitive to the degree of occlusion of tubules, i.e. the presence/absence of a smear layer, than is movement of substances by diffusion. III. BACTERIA IN THE SMEAR LAYER UNDER RESTORATIONS:
whether it should be present or absent under restorations are rather complicated questions. seem
To a great extent they
restorations. ďƒ˜ An invitro study showed that water cleaned cavities with the smear layer remaining underneath the composite restoration showed the presence of numerous bacteria, whereas in the antiseptically cleaned cavities, bacteria were absent. 11
The fact that bacteria multiply on cavity walls even if there is no appreciable communication to the oral cavity seems to indicate
nourishment from the smear layer and dentinal fluid. These considerations favour the opinion that most of the smear
antiseptically treated before the application of lining or a luting cement.
It has also been suggested that bacteria are
not present in freshly prepared smear layers. There is no evidence that common permanent restorative materials
entrapped within the smear layer, especially when a fluid filled
restoration from the smear layer. Bases of 2nOE and Ca(OH) 2 may have good antiseptic effects but
bases cannot be placed on all cavity walls. Pure
dressing and should be applied under temperature fillings. It is also possible but not proved that Ca(OH) 2 may reinforce the remaining smear plugs in the outer apertures of dentinal tubules. IV . THE PROTECTIV E EFFECT OF SMEAR PLUGS IN ** APERTURES AND THE CONSEQUENCE OF REMOV ING THE PLUGS:
In a study 11 years ago they found that etching the cavity prior to the placement of the composite resin resulted in a massive invasion of bacteria in dentinal tubules.
This was 12
cavities, cleaned by water and with smear layer had a bacterial layer on the cavity walls but practically no invasion into the dentinal tubules.
Obviously smear plugs in the
apertures of the tubules had prevented bacterial invasion. Inflammation was present under all infected cavities, being somewhat more pronounced on the etched cavities, but the difference was not great. Thus another conclusion from this study was that smear plugs did not prevent bacterial toxins from diffusing into the pulp. From opened tubules, bacteria may easily reach the pulp and multiply therefore removal of smear plugs should be avoided. Another important consequence of etching and removal of smear plugs and peritubular dentin at the surface is that the area of wet tubules may increase from about 10-25% of the total.
Subsequently it is difficult to get the dentin dry
because fluid continues to be supplied from below through the
adhesive or mechanical bonding to dentin. V. PULPAL IRRITATION DUE TO REMOV AL OF THE SMEAR LAYER:
In several experiments we found that 37% phosphoric acid or 50% citric acid applied for 15 seconds or 1 minute does not result in any appreciable pulpal reaction, inflammation or necrosis. Acid etchants, detergents, a thin mix of phosphate cements, g/c and resin do not produce any appreciable damage and inflammation to the pulp not even when applied to exposed pulp. 13
should not Rxed with acid or EDTA in such a way that the tubules opened are widened. 3. ENDODONTICS: I. ROLE OF SMEAR LAYER IN APICAL LEAKAGE: The smear layer’s presence plays a significant part in an apical
conducive to a better and closer adaptation of the gutta percha to the canal wall with the smear layer intact, apical leakage will be significantly increased without the smear layer, the leakage will still occur but at a decreased rate. Plasticized GP can enter the dentinal tubules when the smear layer is absent.
This can establish a mechanical
block b/w the GP and the canal wall. II. EFFECT OF SMEAR LAYER ON SEALERS: The type of sealer used has different implications once the smear layer is removed.
A powder liquid combination, the
most of which is grossmans sealer contains small particles in the powder that could enter the orifices of the dentinal tubules and help create a reaction interface b/w sealer and canal wall. Ca(OH) 2 based sealers have the advantage of promoting the apposition of cements at the canal apex and sealing it off against microleakage. III. POST CEMENTATION: Removal of smear layer the cementum bond and the tensile strength of the cementing medium.
G/Cs are effective in 14
post cementation after smear layer removal because the glass ionomer has a better union with tooth structure. With the removal of smear layer and an unfilled resin bonding agent, shorter posts can be used. THE SMEAR DILEMMA: The
whether it should be removed or not from the instrumented tooth surface is still contraversial.
The risk of smear layer
acting as a physical barrier to bacteria and its bi-products has been supported by many researchers. Vojinovic et.al. showed that bacteria could not penetrate into dentin in the presence of smear layer. Conversly, Baker and others observed that bacteria could remain in the smear layer and in the dentinal tubule despite instrumentation of the root canal and thus may survive and multiply and grow into dentinal tubules. METHODS OF REMOVAL: Braunsternis group has published several articles describing the use of H2O, H2O21 benzalkonium chloride. other agents to remove the smear layer.
He has formulated
several commercially available products like tubulicid blud label, tubulicid red label etc. that are designed to remove most of smear layer without removing smear debris that has fallen into the orifices of the tubules to form plugs on the cut surface of the dentin. difficult
Though this concept is ideal it is
geometry of many cavities and the difficulty in obtaining adequate access. Remove
especially if dilute acids are used for short periods of time. 15
Etching dentin with 6% citric acid for 60 seconds removes all of the smear layer as does 15 seconds of etching with 37% phosphoric acid. THE ADVANTAGES ARE THAT: •
The smear layer is entirely removed.
The tubules are open and available for retention.
The surface collagen is exposed for possible covalent linkage with new experimental primers for cavities.
Further with the smear layer gone, one does not have to
restoration or being removed by acid produced by bacteria, leaving a void b/w the cavity wall and the restoration might permit bacterial colonization. THE DIS-ADVANTAGES: •
In its absence, there is no physical barrier to bacterial penetration of dentinal tubules. Another entirely different approach would be to use a
resin that would infiltrate through the entire thickness of the smear layer and either bond to underlying matrix or penetrate into the tubules.
The compressive tensile strengths recently
obtained from Scotch bond may be due to such a process. To try to fix the smear layer by gluteraldehyde or tanning agents such as tannic acid or ferric chloride.
The idea is to
increase the cross linking of exposed collagen fibres within the smear layer and b/w it and the matrix of the underlying dentin to improve its cohesion.
The most recent approach to the problem is to remove the smear layer by etching with acid and replace it with an artificial smear layer composed by a crystalline precipitate. Bowen has used this approach by Rxing dentin with 5% ferric oxalate which replaced the original smear layers with a new complex permitting extremely high bond strength to be produced b/w restoration and dentin. The quality of smear layer removed will vary with the type of solvent used. NaOcl: The capacity of NaOcl to remove the smear layer from the instrumented
Even the combination of NaOcl and H2O2
proved to be ineffective.
NaOcl cannot destroy bacteria
within the tubules closed by a smear layer covering. CHELATING AGENTS: The
enthylenediamine tetraactia acid (CEDA 17% 10 minutes) which reacts with Ca++ in dentin and forms soluble calcium chelates.
While Fehr and Nygard Ostry (1963) found that
EDTA decalcified dentin to a depth of 20-30 mm in 5 minutes.
Fraser (1974) stated that chelating effect was
almost negligible in the apical third of the root canals. Different preparations of EDTA have been used as a root canal irrigant.
Root canal preparations i.e. a mixture of
EDTA and urea peroxide left a residue of this mixture after instrumentation.
hermetic sealing of root canals. 17
ammonium bromide) left no smear layer except in the apical part of the canal. GLYOXIDE: Glyoxide is an irrigating solution i.e. comprised of 10% urea peroxide (carbamide peroxide) in a vehicle of anhydrons glycerol.
In 1961 Steward proposed glyoxide to be an
effective adjunct to instrumentation for cleaning of the root canal. It has greater solvent action than 3% H2O2. It enhances root canal lubrication without softening dentin. Other root canal chelating agents are solvizol which is based on
Ceterlon. ORGANIC ACIDS: Citric acid removed smear layer better than many acids such as polyacrylic acid, lactic acid and phosphoric acid and phosphoric
observed that the 25% citric acid – NaOcl combination was not effective as 17% EDTA-NaOcl combination.
citric acid left, precipitated crystals in the root canal which might be dis-advantageous in the root canal obtn. With 50% lactic acid, the canal walls were generally clean but the openings of the dentinal tubules
did not appear
completely patent. 25% tannic acid introduced by Bitter in 1989 was better than NaOcl – H 2 O 2 combination. 18
according to a study conducted by Mc Cough and Smith. NaOcl & EDTA: Goldman et.al. in 1982 have shown that the most effective working solution is 5-25% NaOcl and the most effective final flush was 10 ml of 17% EDTA followed by 10 ml of 5-25% NaOcl.
mineralized dentin, thereby exposing more collagen. ULTRASONICS: Used in conjunction with a solution of NaOcl can eliminate the smear layer.
The apical region of the canal showed less
debris and smear layer than the coronal aspects depending on
magnitude and velocity at the apical region of the file. CONCLUSION: Our knowledge of the smear layer, its structure and function is rapidly growing and will influence all areas of clinical dentistry in the near future. Much more work needs to be done but the promise of greater understanding of the smear layer
dental therapy. REFERENCES: 1. The smear layer in Endodontics, DCNA, January 1990. 2. Operative Dentistry;Suppliment 3,1984 3. Pathways of the Pulp;Cohen